5 2 ( 2 0 1 3 ) 5 6 –6 4
Available at www.sciencedirect.com
journal homepage: www.elsevier.com/locate/carbon
Synthesis and electrochemical performance of reduced graphene oxide/maghemite composite anode for lithium ion batteries Il Tae Kim a, Alexandre Magasinski a, Karl Jacob a, Gleb Yushin
School of Materials Science and Engineering, Georgia Institute of Technology, Atlanta, GA 30332, USA Department of Biomedical Engineering, The School of Medicine and the UAB Comprehensive Cancer Center, University of Alabama at Birmingham, Birmingham, AL 35294, USA
A R T I C L E I N F O
A B S T R A C T
Reduced graphene oxide (rGO) tethered with maghemite (c-Fe2O3) was synthesized using a
Received 5 July 2012
novel modified sol–gel process, where sodium dodecylbenzenesulfonate was introduced
Accepted 1 September 2012
into the suspension to prevent the undesirable formation of an iron oxide 3D network.
Available online 7 September 2012
Thus, nearly monodispersed and homogeneously distributed c-Fe2O3 magnetic nanoparticles could be obtained on surface of graphene sheets. The utilized thermal treatment process did not require a reducing agent for reduction of graphene oxide. The morphology and structure of the composites were investigated using various characterization techniques. As-prepared rGO/Fe2O3 composites were utilized as anodes for half lithium ion cells. The 40 wt.%-rGO/Fe2O3 composite exhibited high reversible capacity of 690 mA h g1 at current density of 500 mA g1 and good stability for over 100 cycles, in contrast with that of the pure-Fe2O3 nanoparticles which demonstrated rapid degradation to 224 mA h g1 after 50 cycles. Furthermore, the composite showed good rate capability of 280 mA h g1 at 10C (10,000 mA g1). These characteristics could be mainly attributed to both the use of an effective binder, poly(acrylic acid) (PAA), and the specific hybrid structures that prevent agglomeration of nanoparticles and provide buffering spaces needed for volume changes of nanoparticles during insertion/extraction of Li ions. Ó 2012 Elsevier Ltd. All rights reserved.
Lithium ion batteries (LIBs) have been widely used as power sources for portable electronic devices and attracted extensive attention due to their high energy density and power density . Anode and cathode materials play important roles in the performance of LIBs. Based on these conceptual approaches, extensive studies have been performed with diverse materials ranging from Si-based anodes with very high gravimetric capacity [2–6] to various transition metal oxides offering high volumetric and moderately high gravimetric capacities [7–17], which is beyond that of commercial
graphitic anodes (340–365 mA h g1, 500–550 mA h cm3), including those based on mesocarbon microbeads (MCMBs), natural graphite and synthetic graphite. The performance of transition metal oxide anodes has commonly been limited due to the high volume changes during continuous charge– discharge process, resulting in breaking down of electrical connection of anode materials from current collectors. Graphene is a two-dimensional aromatic monolayer of carbon atoms with sp2 hybridization. Graphene shows an extraordinary and stable in-plane electrical conductivity, excellent thermal conductivity and mechanical properties, flexible porous structure, and high specific surface area .
* Corresponding authors. E-mail addresses: [email protected]
(G. Yushin), [email protected]
(R. Tannenbaum). 0008-6223/$ - see front matter Ó 2012 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.carbon.2012.09.004
5 2 (2 0 13 ) 5 6–64
Thus, due to these outstanding properties, it has been proposed that graphene could be utilized in energy storage and conversion devices, such as LIBs. As an anode material, graphene has shown a large reversible specific capacity [19– 22]. However, graphene exhibits large irreversible capacity losses, low initial columbic efficiency, and rapid capacity fading. For the purpose of overcoming these limitations and improving electrode capacity and cycling stability, many groups have recently been studying hybrid structures as the anode materials for LIBs such as graphene decorated with such materials as TiO2 , Si , SnO2 , Co3O4 , Fe3O4 [27–29], and Mn3O4 . These hybrid materials have demonstrated large reversible capacity, long cycle life, and good rate performance resulting from new electrochemical behaviors within a confined two-dimensional nanostructure interspaces. Even though some studies on hematite (aFe2O3) were conducted [31, 32], research on another existing abundant form of the iron oxide in nature, maghemite (cFe2O3), have never been reported. Maghemite, c-Fe2O3, is the allotropic form of magnetite, Fe3O4. These two iron oxides are crystallographically isomorphous. The main difference between the two species is the presence of ferric ions only in c-Fe2O3, and both ferrous and ferric ions in Fe3O4. In this paper, we report for the first time on a novel electrode material synthesis approach based on a modified in-situ sol–gel process, which allows uniform attachment of monodispersed oxide nanoparticles to the graphene surface. While the proposed method is applicable for other metal oxides, our proof-of-concept study was focused on the c-Fe2O3 system. For the facile synthesis of reduced graphene oxide/cFe2O3 hybrid structures we utilized an iron salt as a precursor. The transformation of graphene oxide into graphene was accomplished by thermal activation in the absence of a reducing agent. The uniqueness of the proposed synthesis route allowed us to homogeneously tether the maghemite nanoparticles onto the reduced graphene oxide (rGO) sheets and avoid having individual nanoparticles left in the material. Unlike previous studies, which describe efficient and reproducible synthesis methods for the tethering of a-Fe2O3 and Fe3O4 to the surface of graphene [27–29,31,32], our method offers a higher level of control over the nucleation and growth process of the iron oxide nanoparticles on the surface of the graphene. The method is based on a very slow growth of the iron oxide phase, which is controlled by the introduction of the surfactant, preventing the formation of a gel. Moreover, in this system, we do not have to use hydrazine as a reducing agent, since the reduction of graphene oxide is achieved simultaneously during the thermal treatment leading to the formation of the c-Fe2O3 nanoparticles. The proposed procedure guaranteed that all the nanoparticles maintain electrical connectivity during large volume changes and assist in avoiding agglomeration during continuous charge–discharge processes. Moreover, the tethered maghemite nanoparticles greatly assist in keeping adjacent graphene sheets separated and avoiding re-stacking of graphene sheets into graphite. In a previous study, we reported poly(acrylic acid) (PAA) as an efficient binder for Si anode . Here we demonstrate the effective use of PAA in rGO/c-Fe2O3 composites. PAA is soluble in water as well as in a variety of ecologically friendly organic solvents such as ethanol. PAA can interact with copper
surface via hydrogen bonding (with Cu oxide) and/or Cu salt formation; namely, PAA has good adhesion strength between the electrode and the current collector foil for the integrity of the anode. In addition, as-prepared PAA films showed negligible swellability in the carbonate vapors (DEC vapor), resulting in a low level interaction of PAA/electrolyte and retention of mechanical properties, contrary to those of polyvinylidene fluoride (PVDF). The rGO/c-Fe2O3/PAA composite anode showed excellent cycling performance and rate capability even at high current rate of 10C. Therefore, functionalizing graphene sheets with iron oxide nanoparticles and using an effective binder, PAA, may promise as a future electrode system for lithium ion batteries with superior energy and power density.
2.1. Preparation of reduced graphene oxide (rGO)–Fe2O3 hybrid structure Graphite oxide (GO) was synthesized from natural graphite flakes (325 mesh, 99.8% metal basis) purchased from Alfa Aesar by applying a modified Hummers method . In brief, graphite powder (2 g) and sodium nitrate (NaNO3, 1 g) were mixed with concentrated sulfuric acid (H2SO4, 70 mL) under stirring and cooled by using an ice bath. Potassium permanganate (KMnO4, 6 g) was added gradually under vigorous stirring, while keeping the temperature of the mixture below 20 °C. Successively, the mixture was intensely stirred at 35 ± 3 °C for 30 min, resulting in the formation of a thick paste. Next, 150 mL of DI water was slowly added, and the solution was stirred for 15 min at 90 ± 3 °C. After dilution with 240 mL of DI water, 5 mL of hydrogen peroxide (H2O2, 30%) was added to the mixture and stirred for 2 h, turning the color of the solution from the dark brown to brilliant yellow accompanied by bubbling. After that, the mixture was filtered and washed with 250 mL of hydrochloric acid (HCl, 10%), followed by DI water until the pH of the supernatant was neutral. Finally, the resulting solid was dried in a vacuum. Reduced graphene oxide (rGO)–Fe2O3 hybrid materials were synthesized by applying a novel synthesis technique, modified sol–gel process. The synthesis of rGO–Fe2O3 was performed by first adding 0.65 g Fe(NO3)3Æ9H2O to 20 ml of DI water and stirring until the Fe(NO3)3Æ9H2O was dissolved completely. Subsequently, GO was added to the solution with a mass ratio of 4:1 (Fe(NO3)3Æ9H2O:GO mass ratio of 4:1), stirred, and ultra-sonicated for 3 h. For the preparation of sample with 8:1 mass ratio, 1.3 g of Fe(NO3)3Æ9H2O was added. Twenty milliliter of 1.2 mM of NaDDBS (sodium dodecyl benzene sulfonate) was added to the solution and stirred for 30 min. Then, 1.2 ml of propylene oxide was added as a gelation agent and stirred for 30 min. The mixture was then placed in a Fisher Scientific iso-temperature oven for drying for 3 days at 100 °C. The resulting powder products were washed with DI water and ethanol and centrifuged several times. In this step, the supernatant, including unreacted iron ions and dissolved iron hydroxide molecules was decanted repeatedly until the its color changed from bright yellow to clear, in order to obtain only GO/iron oxide hybrids. After that, the remaining
5 2 ( 2 0 1 3 ) 5 6 –6 4
Fig. 1 – Schematic representation of overall strategy for producing rGO–Fe2O3 hybrid structures.
powder samples were dried at 50 °C. The calcination of these powders was performed in a furnace under argon atmosphere at 500 °C for 2 h. The schematic illustration is shown in Fig. 1. For the preparation of pure Fe2O3 nanoparticles, the synthesis was the same as the previously conducted process, in the absence of GO. The nanoparticle size of pure Fe2O3 was approximately 30 nm (Fig. S1).
(PP/PE/PP) membrane (Celgard 2325) was used as a separator. Galvanostatic charge–discharge cycling was performed on an Arbin SB2000 (Arbin Instrument, USA) in the range of 0.01–3.0 V. Cyclic voltammetry in the potential window of 0.01–3.0 V at a scan rate of 0.014 mV s1 was performed on a Solartron 1480 (Solartron Analytical, USA) multichannel potentiostat.
X-ray diffraction (XRD) measurements were performed with ˚ ). XRD peaks were an X’pert Pro Alpha-1 (wavelength of 1.54 A collected from 2h = 8° to 70° with a step size of 0.02°. The morphology of as-prepared samples was characterized using SEM (LEO 1530). TEM samples were prepared by placing a droplet of solution onto a TEM grid. These samples were analyzed using a Hitachi HF2000, 200 kV transmission electron microscope. XPS scans of powder samples were taken using a Surface Science Laboratories SSX-100 ESCA spectrometer using monochromatic Al Ka radiation (1486.6 eV). Thermal gravimetric analysis (TGA) using a Q50, TA Instrument, was used with a heating rate of 10 °C min1 from room temperature to 800 °C under both nitrogen and air atmosphere. N2 physisorption (Micromeritics TriStar II 3020) at 196 °C allowed for the determination of the specific surface area of the as-prepared materials. Each sample was degassed in N2 gas at 100 and 300 °C for at least 30 min and 8 h, respectively, prior to the measurements. The Brunauer–Emmett–Teller method was used to calculate the surface area.
Electrodes were prepared by mixing rGO–Fe2O3 nanocomposites, Pure blackâ, polyacrylic acid (Mw: 450 kDa) with the weight ratio of 85:5:10 in water to form a slurry. As-prepared slurry was cast on a 18 lm Cu foil (Fukuda, Japan), dried in air at room temperature first, and then dried in vacuum at 70 °C overnight. The commercial electrolyte consists of 1 M LiPF6 salt in ethylene carbonate–diethyl carbonate–dimethyl carbonate mixture (EC:DEC:DMC = 1:1:1 vol%) (Novolyte Technologies, USA). 2.5 wt.% of vinylene carbonate (VC; Alfa Aesar, USA) was added into the electrolyte solution. Lithium metal foil (0.9 mm thick, Alfa Aeasr, USA) was used as a reference electrode. 2016 type coin cells were used for electrochemical characterizations and assembled in an argon-filled glove box (<1 ppm H2O, O2). The Cu current collector of the working electrode was spot-welded to the coin cell for enhancing electrical contact. A polyethylene–polypropylene–polyethylene
Results and discussion
3.1. Characterization of reduced graphene oxide (rGO)–Fe2O3 nanocomposites Fig. 2 shows the X-ray diffraction patterns of graphite, graphene oxide (GO), and rGO–Fe2O3 hybrid structures. Compared with the pristine graphite, the diffraction peak of GO appears at 10.9° (0 0 2) since the AB stacking order is still observed in graphite oxide with the d-spacing of 0.813 nm . This shows larger value than the d-spacing (0.335 nm) of pristine graphite (2h = 26.6°) due to the intercalated water molecules between
2θ (degree) Fig. 2 – X-ray diffraction patterns of (a) graphite, (b) GO, and (c) rGO–Fe2O3 nanocomposites.
layers [35–37]. After being tethered with Fe2O3 through a calcination process, graphene oxide was reduced without using additional reduction agents as shown in Fig. 2(c). The scanning electron microscope (SEM) and high-resolution transmission electron spectroscope (HRTEM) images of GO and rGO–Fe2O3 nanocomposites are shown in Fig. 3. Fig. 3a shows the TEM image of GO. Fig. 3(b) and (c) show
the synthesized rGO–Fe2O3 with the mass ratio of 4:1 (Fe(NO3)3Æ9H2O:GO mass ratio of 4:1). From the TGA result (Fig. S2), the weight fraction of rGO was 40 wt.%. In addition, Fig. 3(d) shows the TEM image of rGO–Fe2O3 nanocomposite with the mass ratio of 8:1, where the weight fraction of rGO from the TGA result was 27.5%. The surfaces of the rGO sheets were homogeneously tethered with Fe2O3 nanoparticles and
C-C (284.6 eV)
(f) Intensity (a. u.)
C-O (286.7 eV)
5 2 (2 0 13 ) 5 6–64
C(O)O (288.7 eV)
Binding Energy (eV)
Binding Energy (eV)
Fig. 3 – (a) TEM image of GO; inset shows the diffraction pattern. (b) SEM image and (c) TEM image of 40 wt.%-rGO–Fe2O3 hybrid structure. (d) TEM image of 27.5 wt.%-rGO–Fe2O3 hybrid structure. XPS spectra of C1s of (e) GO and (f) rGO–Fe2O3 hybrid materials.
5 2 ( 2 0 1 3 ) 5 6 –6 4
Quantity Adsorbed (cm3/g STP)
the nanoparticle sizes of 40 wt.% and 27.5 wt.%-rGOs were approximately 15 and 28 nm, respectively. By increasing the concentration of iron salts, the size and density of nanoparticles on the graphene sheets increased as well. The insets in Fig. 3(a) and (c) show the diffraction patterns, illustrating well-defined crystal structures of graphene and tethered nanoparticles. These as-prepared hybrid composite materials exhibit uneven and rough surface characteristics with large amount of void spaces, which would affect the electrochemical performance when these are used as anode materials for lithium ion batteries. Fig. 3(e) and (f) show X-ray photoelectron spectroscopy (XPS) spectra of GO and rGO–Fe2O3 composite materials. The C1s spectrum of GO shows two main peaks centered at 284.6 and 286.7 eV, which correspond to the binding energy of sp2 C–C bonds and C–O bonds in the epoxy/hydroxyl/carbonyl groups. In comparison to the C1s spectrum of GO, the spectrum of rGO–Fe2O3 shows a strong peak corresponding to sp2 C–C bonds, demonstrating the reduction of functionalized groups containing oxygen during the thermal process [38,39]. The porous structure features and Brunauer–Emmett–Teller (BET) specific surface area of 40 wt.%-rGO–Fe2O3 and 27.5 wt.%-rGO–Fe2O3 composite materials were investigated by N2 adsorption/desorption isotherms as shown in Fig. 4. When we compare BET specific surface area for composite materials, the value of 40 wt.%-rGO–Fe2O3 is 81 m2 g1, which is larger than that (64 m2 g1) of 27.5 wt.%-rGO–Fe2O3 composite material. This is good agreement with the TEM images. In the case of 40 wt.%-rGO–Fe2O3, the tethered nanoparticle size was smaller than that of 27.5 wt.%-rGO–Fe2O3; thus, the latter exhibits the lower specific surface area. The relatively large specific surface area is beneficial for the electrolyte access, but, unfortunately, increases irreversible capacity losses at the first cycle due to the electrolyte decomposition and solid electrolyte interphase (SEI) formation. The total pore volumes of 40 wt.%-rGO–Fe2O3 and 27.5 wt.%-rGO–Fe2O3 composite materials are 0.21 and 0.18 cm3 g1, respectively. The nanopores in composite materials could tolerate the volume changes of Fe2O3 nanoparticles during intercalation/deintercalation process of lithium ions and may affect the large capacity, good rate performance, and cycling stability [29,40,41].
40 wt% rGO-Fe2 O3 - Adsorption
40 wt% rGO-Fe2 O3 - Desorption 27.5 wt% rGO-Fe2 O3 - Adsorption
27.5 wt% rGO-Fe2 O3 - Desorption
80 60 40 20 0 0.0
Relative Pressure (P/Po) Fig. 4 – N2 adsorption/desorption isotherms of 40 wt.%-rGO– Fe2O3 and 27.5 wt.%-rGO–Fe2O3 hybrid materials.
3.2. Electrochemical performance nanocomposites and Fe2O3 nanoparticles
The electrochemical properties of the rGO–Fe2O3 nanocomposites and the pure-Fe2O3 nanoparticles were compared and investigated. Intercalation/deintercalation cycling of Li ions was carried out in the voltage range of 0.01–3.0 V. The intercalation/deintercalation curves for as-prepared 40 wt.%rGO–Fe2O3 nanocomposite and pure-Fe2O3 are shown in Fig. 5(a) and (b). The first two intercalation/deintercalation cycles were tested at a current density of 45 mA g1, and next up to 100th cycle after first two cycles was conducted at a current density of 500 mA g1. In the first cycle, the intercalation/ deintercalation capacities of as-prepared pure-Fe2O3 were 1032 and 755 mA h g1, respectively. However, it fades quickly as shown in Fig. 5(b) due to the severe aggregation and high volume changes of Fe2O3 nanoparticles during Li+ insertion/ extraction process [42,43]. Such aggregations combined with large volume changes may destroy the SEI layer, which, in turn, consumes Li ions and leads to poor cyclic performances. On the contrary, the first intercalation voltage profile of the rGO–Fe2O3 nanocomposite is very similar to that of rGO– Fe3O4 nanocomposites reported [44–46]. The maghemite, cFe2O3, is the allotropic form of magnetite, Fe3O4. These two iron oxides are crystallographically isomorphous. Thus, we could expect that our new composite system may show similar tendency. In the first intercalation curve as shown in Fig. 5(a), two voltage plateaus at 0.95 and 0.8 V were observed. The voltage plateau at 0.95 V can be attributed to the irreversible reaction. On the other hand, the plateau at 0.8 V reflects the reduction of Fe(III) to Fe(0). The deintercalation curve showed a sloping plateau at 1.6 V due to the reverse reaction. The 40 wt.%-rGO–Fe2O3 electrode showed an initial discharge capacity of 1133 mA h g1 and charge capacity of 782 mA h g1 in the first cycle; thus, Coulombic efficiency was about 70%. This irreversible capacity observed in the first cycle may be caused by the formation of solid electrolyte interphase (SEI) film, the decomposition of electrolyte, and the conversion of Fe2O3 to Fe nanoparticles along with the formation of amorphous Li2O [10,19,27,29,47,48]. It may be also caused by the interaction of Li ions with the vacant spaces in octahedral positions of the crystal structure of maghemite [49–51]. During the second cycle, the intercalation capacity decreased to 804 mA h g1, leading to a much higher Coulombic efficiency of 96.3%. Furthermore, when we increased the current density to 500 mA g1 from the 3rd cycle, the intercalation and deintercalation capacities of the hybrid material were 663 and 649 mA h g1 in 3rd cycle, 649 and 637 mA h g1 in 4th cycle, respectively. The Coulombic efficiencies of those cycles were close to 100%. To identify all of the electrochemical reactions, cyclic voltammetry (CV) was conducted on the cell with 40 wt.%-rGO– Fe2O3 at room temperature in the 0.01–3.0 V range and a scan rate of 0.014 mV s1 as shown in Fig. 5(c). In the first cycle, the peak is observed at 0.95 V, which can be attributed to the reduction of the irreversible reaction with the electrolyte. The peak observed at 0.75 V can be ascribed to the lithiation reaction of Fe2O3 with Li ions as following [31,52]: þ
Fe2 O3 þ 6Li þ 6e () 2Fe þ 3Li2 O
5 2 (2 0 13 ) 5 6–64
4th 3rd 50th
C/20 2nd 1st
2.5 2.0 1.5
Capacity (mA h g )
Capacity (mA h g )
(c) Current (mA)
-0.05 3rd 2nd
Voltage (V) vs. Li/Li
Fig. 5 – Intercalation/deintercalation curves of (a) 40 wt.%-rGO–Fe2O3 and (b) pure-Fe2O3 nanoparticles at current density of 45 mA g1 (0.05 C) and 500 mA g1 (0.5 C). (c) Cyclic voltammogram of 40 wt.%-rGO–Fe2O3 composite at a scan rate of 0.014 mV s1.
Meanwhile, two peaks were recorded at about 1.56 and 1.85 V in the anodic process, which correspond to the oxidation of Fe0 to Fe3+. During the subsequent cycles, the cathodic and anodic peaks are positively shifted, which is attributed to the polarization of the electrode in the first cycle. Moreover, a decrease of the redox peak intensity from the 1st cycle to 2nd cycle implies that the capacity is decreased. However, after first cycling, both the peak current and the integrated area of their anodic peaks are changeless, indicating no capacity loss during the delithiation process. The intercalation/deintercalation cycling performance of the as-prepared 40 wt.%-rGO–Fe2O3, 27.5 wt.%-rGO/Fe2O3, and pure-Fe2O3 were evaluated between 0.01 and 3.0 V at 0.05C (first two cycles) and 0.5C as shown in Fig. 6(a). In the first cycle, the intercalation capacity of the pure-Fe2O3 nanoparticle electrode is about 1032 mA h g1. However, the capacity continuously decreases and reaches 224 mA h g1 after 50 cycles, which is only about 22% of the initial capacity, illustrating poor capacity retention. In the case of hybrid materials, rGO–Fe2O3 nanocomposites, the first cycle capacities of both 40 wt.%-rGO–Fe2O3 and 27.5 wt.%-rGO–Fe2O3 at current density of 45 mA g1, were 1132 and 1059 mA h g1, respectively. After 50th cycle, the capacities at current density of 500 mA g1, were 666 and 575 mA h g1, respectively, and they
still marked 59% and 54% of the initial capacity. Importantly, we investigated the binder efficiency on cycling performance by using PAA and PVDF at the current density of 500 mA g1 for 40 wt.%-rGO–Fe2O3 composite electrode. As shown in Fig. 6(b), rGO/Fe2O3/PVDF composite anode showed similar cyclability with that of rGO/Fe2O3/PAA composite anode in the earlier cycles. However, by undergoing charge/discharge process, rGO/Fe2O3/PVDF composite anode showed capacity fading. On the other hand, when rGO/Fe2O3/PAA composite anode was tested, it exhibited excellent cyclic performance, retained 690 mA h g1 capacity, and showed Coulombic efficiency of above 99%. To further investigate the electrochemical performance of the hybrid composite materials and pure-Fe2O3 nanoparticles, the rate capability of the samples were conducted as shown in Fig. 6(c). In the case of pure-Fe2O3 electrode, it showed reasonable capacities from current density, 0.1C to 1C. However, at high current density, for example, 2C, 5C, or 10C, its values are very low. When we observe the results of as-prepared samples, 40 wt.%-rGO–Fe2O3 and 27.5 wt.%-rGO–Fe2O3 composite electrodes, they showed higher capacity than that of pure-Fe2O3 nanoparticle electrode. Specifically, in the case of 40 wt.%-rGO–Fe2O3 composite electrode, it showed better capacity retention about 380 mA h g1, even at high current
600 27.5 wt%-rGO-Fe2O3
400 75 pure-Fe2O3
Coulombic efficiency (%)
Capacity (mA h g )
5 2 ( 2 0 1 3 ) 5 6 –6 4
rGO/Fe2O3 with PAA
500 mA g
600 80 400 rGO/Fe2O3 with PVDF
Coulombic efficiency (%)
Capacity (mA h g-1)
40 wt%-rGO-Fe2O3 27.5 wt%-rGO-Fe2O3
Capacity (mA h g )
C/5 C/2 1C
600 2C 5C
200 0 0
Cycle number Fig. 6 – (a) Cycle performance of the 40 wt.%-rGO–Fe2O3, 27.5 wt.%-rGO–Fe2O3, and pure-Fe2O3 electrodes at current rates of 0.05 C (first two cycles) and 0.5 C. (b) Cycle performance of the 40 wt.%-rGO–Fe2O3 composites with different binder at a current density of 500 mA g1 for 100 cycles. (c) The rate performance of the 40 wt.%-rGO–Fe2O3, 27.5 wt.%-rGO–Fe2O3, and pure-Fe2O3 electrodes at different current densities.
density of 5C. Furthermore, we compared our results for rate performance to those of similar graphene/iron oxide composite anodes reported before, which is summarized in Table 1. Each reported material has different synthesis method, and indicated capacities (mA h g1) from other reports are rough values. As shown in Table 1, current work (40 wt.%-rGO/ Fe2O3/PAA) show better rate performance; especially, at high current rates (5C and 10C), this material shows excellent values. These results clearly show that the well-organized flexible intercalated structure plays an important role in improving the electrochemical performance. Fe2O3 nanoparti-
cles tethered homogeneously on the graphene sheets result in the dimensional confinement of the Fe2O3 nanoparticles, limiting the effect of volume expansion during lithiation due to the enough void spaces between graphene sheets. Furthermore, graphene sheets serve not only as an efficient conducting matrix for maintaining the structural integrity of the electrode during insertion/extraction process of Li ions, but also as an enduring agent preventing nanoparticles tethered on graphene sheets from aggregating and resulting in the release of the stress that arises during the process of Li+ insertion/extraction.
Table 1 – Summary of rate performance (mA h g1) of graphene/iron oxide composites. C rate Components
G/Fe3O4 G/Fe3O4 G/Fe3O4 G/Fe3O4 G/Fe3O4 G/Fe3O4 G/a-Fe2O3 G/c-Fe2O3current
– 870 640 1048 890 – 831
539 730 830 – – 870 – 818
470 580 – 430 600 710 653 690
340 510 610 350 410 700 595 656
220 380 520 280 – 540 – 510
100 190 – 170 – 350 456 380
– – – – – – 215 280
5 2 (2 0 13 ) 5 6–64
In summary, our modified sol–gel technique for developing reduced graphene oxide/iron oxide hybrid structures was successfully utilized, where individual and homogeneouslydistributed maghemite, c-Fe2O3, were synthesized and tethered onto the surface of graphene sheets. The reduced graphene oxide/Fe2O3 nanocomposite electrodes exhibit improved reversible capacity, cycle life, and good rate capability. These enhancements can be ascribed to specific hybrid structures, which have significant roles such as the formation of the efficient electrically conductive networks, the inhibition of aggregation of adjacent Fe2O3 nanoparticles, and the offer of the buffering spaces against extreme volume changes of Fe2O3 nanoparticles during continuous intercalation/deintercalation process of Li ions. In addition, we found PAA to acts as a very efficient binder for graphene oxide/Fe2O3 based electrodes. Reduced graphene oxide/Fe2O3 composite electrode maintains a high reversible capacity of 690 mA h g1 up to the 100th cycle even at high current density of 500 mA g1, showing highly enhanced cycle performance compared to that of pure-Fe2O3 nanoparticles. Therefore, the developed process for the formation of graphene sheets tethered with transition metal oxides offers a great potential for the formation of electrode materials for energy storage systems, such as lithium ion batteries and supercapacitors.
Acknowledgements Il Tae Kim was supported by Paper Science and Engineering (PSE) Graduate Fellowships from the Institute of Paper Science and Technology (IPST) at the Georgia Institute of Technology. G. Yushin and A. Magasinski were supported by the Energy Efficiency & Resources program of the Korea Institute of Energy Technology Evaluation and Planning (KETEP) Grant 20118510010030.
Appendix A. Supplementary data Supplementary data associated with this article can be found, in the online version, at http://dx.doi.org/10.1016/j.carbon. 2012.09.004.
R E F E R E N C E S
 Tarascon JM, Armand M. Issues and challenges facing rechargeable lithium batteries. Nature 2001;414(6861):359–67.  Magasinski A, Dixon P, Hertzberg B, Kvit A, Ayala J, Yushin G. High-performance lithium-ion anodes using a hierarchical bottom-up approach. Nat Mater 2010;9(4):353–8.  Magasinski A et al. Toward efficient binders for Li-ion battery Si-based anodes: polyacrylic acid. ACS Appl Mater Interfaces 2010;2(11):3004–10.  Kovalenko I, Zdyrko B, Magasinski A, Hertzberg B, Milicev Z, Burtovyy R, et al. A major constituent of brown algae for use in high-capacity Li-ion batteries. Science 2011;334(6052):75–9.
 Evanoff K, Magasinski A, Yang J, Y G. Nano Si-coated graphene granules as anodes for Li-ion batteries. Adv Energy Mater 2011;1(4):495–8.  Hertzberg B, Alexeev A, Yushin G. Deformations in Si–Li anodes upon electrochemical alloying in nano-confined space. J Am Chem Soc 2010;132(25):8548–9.  Li YG, Tan B, Wu YY. Mesoporous CO3O4 nanowire arrays for lithium ion batteries with high capacity and rate capability. Nano Lett 2008;8(1):265–70.  Lou XW, Wang Y, Yuan CL, Lee JY, Archer LA. Template-free synthesis of SnO2 hollow nanostructures with high lithium storage capacity. Adv Mater 2006;18(17):2325.  Poizot P, Laruelle S, Grugeon S, Dupont L, Tarascon JM. Nanosized transition-metaloxides as negative-electrode materials for lithium-ion batteries. Nature 2000;407(6803):496–9.  Reddy MV, Yu T, Sow CH, Shen ZX, Lim CT, Rao GVS, et al. alpha-Fe2O3 nanoflakes as an anode material for Li-ion batteries. Adv Funct Mater 2007;17(15):2792–9.  Zhi LJ, Hu YS, El Hamaoui B, Wang X, Lieberwirth I, Kolb U, et al. Precursor-controlled formation of novel carbon/metal and carbon/metal oxide nanocomposites. Adv Mater 2008;20(9):1727.  Qiao H, Xiao LF, Zheng Z, Liu HW, Jia FL, Zhang LZ. One-pot synthesis of CoO/C hybrid microspheres as anode materials for lithium-ion batteries. J Power Sources 2008;185(1):486–91.  Wu XL, Guo YG, Wan LJ, Hu CW. Alpha-Fe2O3 nanostructures: inorganic salt-controlled synthesis and their electrochemical performance toward lithium storage. J Phys Chem C 2008;112(43):16824–9.  Xiang JY, Tu JP, Zhang L, Zhou Y, Wang XL, Shi SJ. Simple synthesis of surface-modified hierarchical copper oxide spheres with needle-like morphology as anode for lithium ion batteries. Electrochim Acta 2010;55(5):1820–4.  Yuan L, Guo ZP, Konstantinov K, Munroe P, Liu HK. Spherical clusters of NiO nanoshafts for lithium-ion battery anodes. Electrochem Solid State Lett 2006;9(11):A524–8.  Chen LB, Lu N, Xu CM, Yu HC, Wang TH. Electrochemical performance of polycrystalline CuO nanowires as anode material for Li ion batteries. Electrochim Acta 2009;54(17):4198–201.  Cui ZM, Hang LY, Song WG, Guo YG. High-yield gas–liquid interfacial synthesis of highly dispersed Fe3O4 nanocrystals and their application in lithium-ion batteries. Chem Mater 2009;21(6):1162–6.  Geim AK, Novoselov KS. The rise of graphene. Nat Mater 2007;6(3):183–91.  Guo P, Song HH, Chen XH. Electrochemical performance of graphene nanosheets as anode material for lithium-ion batteries. Electrochem Commun 2009;11(6):1320–4.  Pan DY, Wang S, Zhao B, Wu MH, Zhang HJ, Wang Y, et al. Li storage properties of disordered graphene nanosheets. Chem Mater 2009;21(14):3136–42.  Wang GX, Shen XP, Yao J, Park J. Graphene nanosheets for enhanced lithium storage in lithium ion batteries. Carbon 2009;47(8):2049–53.  Yoo E, Kim J, Hosono E, Zhou H, Kudo T, Honma I. Large reversible Li storage of graphene nanosheet families for use in rechargeable lithium ion batteries. Nano Lett 2008;8(8):2277–82.  Kim HK, Bak SM, Kim KB. Li4Ti5O12/reduced graphite oxide nano-hybrid material for high rate lithium-ion batteries. Electrochem Commun 2010;12(12):1768–71.  Evanoff K, Magasinski A, Yang J, Yushin G. Nanosiliconcoated graphene granules as anodes for Li-ion batteries. Adv Energy Mater 2011;1(4):495–8.  Paek SM, Yoo E, Honma I. Enhanced cyclic performance and lithium storage capacity of SnO2/graphene nanoporous
  
5 2 ( 2 0 1 3 ) 5 6 –6 4
electrodes with three-dimensionally delaminated flexible structure. Nano Lett 2009;9(1):72–5. Yang SB, Feng XL, Wang L, Tang K, Maier J, Mullen K. Graphene-based nanosheets with a sandwich structure. Angew Chem-Int Ed 2010;49(28):4795–9. Wang JZ, Zhong C, Wexler D, Idris NH, Wang ZX, Chen LQ, et al. Graphene-encapsulated Fe3O4 nanoparticles with 3D laminated structure as superior anode in lithium ion batteries. Chem – Eur J 2011;17(2):661–7. Zhang M, Lei DN, Yin XM, Chen LB, Li QH, Wang YG, et al. Magnetite/graphene composites: microwave irradiation synthesis and enhanced cycling and rate performances for lithium ion batteries. J Mater Chem 2010;20(26):5538–43. Zhou GM et al. Graphene-wrapped Fe3O4 anode material with improved reversible capacity and cyclic stability for lithium ion batteries. Chem Mater 2010;22(18):5306–13. Wang HL, Cui LF, Yang YA, Casalongue HS, Robinson JT, Liang YY, et al. Mn3O4–graphene hybrid as a high-capacity anode material for lithium ion batteries. J Am Chem Soc 2010;132(40):13978–80. Zhu XJ, Zhu YW, Murali S, Stollers MD, Ruoff RS. Nanostructured reduced graphene oxide/Fe2O3 composite as a high-performance anode material for lithium ion batteries. ACS Nano 2011;5(4):3333–8. Zhu JX et al. Facile synthesis of metal oxide/reduced graphene oxide hybrids with high lithium storage capacity and stable cyclability. Nanoscale 2011;3(3):1084–9. Hummers WSO, E R. Preparation of graphitic oxide. J Am Chem Soc 1958;80(6):1339. Jeong HK et al. Evidence of graphitic AB stacking order of graphite oxides. J Am Chem Soc 2008;130(4):1362–6. Buchsteiner A, Lerf A, Pieper J. Water dynamics in graphite oxide investigated with neutron scattering. J Phys Chem B 2006;110(45):22328–38. Hontorialucas C, Lopezpeinado AJ, Lopezgonzalez JDD, Rojascervantes ML, Martinaranda RM. Study of oxygencontaining groups in a series of graphite oxides - physical and chemical characterization. Carbon 1995;33(11):1585–92. Guo HL, Wang XF, Qian QY, Wang FB, Xia XH. A green approach to the synthesis of graphene nanosheets. ACS Nano 2009;3(9):2653–9. Ha HW, Kim IY, Hwang SJ, Ruoff RS. One-pot synthesis of platinum nanoparticles embedded on reduced graphene oxide for oxygen reduction in methanol fuel cells. Electrochem Solid State Lett 2011;14(7):B70–3. Stankovich S et al. Synthesis of graphene-based nanosheets via chemical reduction of exfoliated graphite oxide. Carbon 2007;45(7):1558–65.
 Yang SB, Cui GL, Pang SP, Cao Q, Kolb U, Feng XL, et al. Fabrication of cobalt and cobalt oxide/graphene composites: towards high-performance anode materials for lithium ion batteries. Chemsuschem 2010;3(2):236–9.  He Y, Huang L, Cai JS, Zheng XM, Sun SG. Structure and electrochemical performance of nanostructured Fe3O4/ carbon nanotube composites as anodes for lithium ion batteries. Electrochim Acta 2010;55(3):1140–4.  Muraliganth T, Murugan AV, Manthiram A. Facile synthesis of carbon-decorated single-crystalline Fe3O4 nanowires and their application as high performance anode in lithium ion batteries. Chem Commun 2009(47):7360–2.  Zhang WM, Wu XL, Hu JS, Guo YG, Wan LJ. Carbon coated Fe3O4 nanospindles as a superior anode material for lithiumion batteries. Adv Funct Mater 2008;18(24):3941–6.  Ji LW, Tan ZK, Kuykendall TR, Aloni S, Xun SD, Lin E, et al. Fe3O4 nanoparticle-integrated graphene sheets for highperformance half and full lithium ion cells. Phys Chem Chem Phys 2011;13(15):7139–46.  Li BJ, Cao HQ, Shao J, Qu MZ, Warner JH. Superparamagnetic Fe3O4 [email protected]
composites for energy storage devices. J Mater Chem 2011;21(13):5069–75.  Lian PC, Zhu XF, Xiang HF, Li Z, Yang WS, Wang HH. Enhanced cycling performance of Fe3O4–graphene nanocomposite as an anode material for lithium-ion batteries. Electrochim Acta 2010;56(2):834–40.  Liu H, Wang GX, Wang JZ, Wexler D. Magnetite/carbon coreshell nanorods as anode materials for lithium-ion batteries. Electrochem Commun 2008;10(12):1879–82.  Ban CM, Wu ZC, Gillaspie DT, Chen L, Yan YF, Blackburn JL, et al. Nanostructured Fe3O4/SWNT electrode: binder-free and high-rate Li-ion anode. Adv Mater 2010;22(20):E145.  deFaria DLA, Silva SV, deOliveira MT. Raman microspectroscopy of some iron oxides and oxyhydroxides. J Raman Spectrosc 1997;28(11):873–8.  Millan A et al. Maghemite polymer nanocomposites with modulated magnetic properties. Acta Mater 2007;55(6):2201–9.  White WB, Deangeli Ba. Interpretation of vibrational spectra of spinels. Spectrochim Acta A: Mol Spectrosc 1967;A 23(4):985.  Yuan SM, Zhou Z, Li G. Structural evolution from mesoporous alpha-Fe2O3 to [email protected]
and gamma-Fe2O3 nanospheres and their lithium storage performances. CrystEngComm 2011;13(14):4709–13.